Iraqi Journal of Applied Physics Abdulghefar K. Faiq Department of Physics, College of Science, University of Salahaddin, Erbil, Kurdistan Region, Iraq Extraction of Doping Profile in Substrate of MNOS capacitor Using Fast Voltage Ramp Deep Depletion C-V method Two MNOS C-V profiling methods are presented; the conventional C-V profiling, and deep depletion (DD) C-V, the former shows a lack of information at the onset of inversion mode, while the latter can be achieved by the application of high speed voltage ramp of sweep rate equals 1MV/s on the MNOS gate, meanwhile monitoring the current response of the time varying voltage, the entire DD C-V curve is traced on CRO screen with suitable DC voltage bias. The results show that doping profile can be extended 1µm deeper inside the silicon, i.e., ten times of Debye's length, hence more accurate results can be achieved. Interface states densities have small effect on final doping profile, and doping reaches approximately a constant value deep inside the silicon compatible with experimental part. Keywords: Semiconductor devices, Doping profiling, MNOS, Deep depletion Received: 30 October 2009, Revised: 4 March 2010, Accepted: 11 March 2010 1. Introduction Metal-Nitride-Oxide-Semiconductor (MNOS) capacitor is the essential part in nonvolatile memory, it is also used as a passive coating due to its high resistivity, and higher dielectric constant compared to silicon dioxide [1,2]. The calculation of doping profile is important to understand the characteristics of shrunken device, such as the device conductivity which is very sensitive to doping variation near the silicon substrate [1,3]. There are several methods to extract impurity distribution pattern, the simplest, and the non–destructive one is the Capacitance-Voltage (C-V) method [4]. Over the years many researches on C-V profiling has, in general, remained limited to MOS [5]. In this work we try, to examine the suitability of C-V technique to deduce doping distribution under the oxide of MNOS structure, and to obtain deep depletion C-V curve in such devices in order to extend the profile deep inside the silicon substrate. The C-V profiling is essentially a measurement of free hole concentration p(x) -for p-type silicon- rather than of the real doping concentration Na(x) of semiconductor. Whenever space charge are present, the two are not the same, but deep inside the semiconductor substrate, p(x) will eventually become flat, and p(x) 0 Na(x) [6]. It is worth to note that in spite of the above mentioned limitation concerning the validity of the C-V profiling, this technique proves to be very useful for determining various doping profiles in semiconductors [7]. All rights reserved 2. Theoretical bases The typical MNOS structure and its C-V curves at low frequency, high frequency, and deep depletion (DD) are shown in Fig. (1). C-V curves span the accumulation to the depletion modes [8]. The capacitance of MNOS structure at high frequency can be represented by two capacitors in series [9]: (1) The insulator capacitance (Ci ) which in turn is composed of a series combination of two capacitances; silicon nitride capacitance (Cn), and silicon dioxide capacitance (Co). (2) The silicon depletion-region capacitance Cd. In our MNOS structure, the oxide thickness is 2nm and silicon nitride thickness is 171nm, the Ci of MNOS structure is given by: CC (1) Ci = o n Co + Cn Co = (2) ox o do where ox is the relative dielectric constant of silicon dioxide (=3.9) and do its thickness Cn = (3) n o dn where n is the relative dielectric constant of silicon nitride which is between 6 and 7 [10], and dn is the nitride layer thickness ISSN 1813-2065 Printed in IRAQ 35 IJAP Vol. (6), No. (1), January 2010 This equation shows that the doping concentration N(w) can be calculated from the slope of (1/Cm2) vs. V curve. The above relation is considered to be the free carrier concentration, more specifically, when the true hole concentration p(x) varies by an appreciable fraction over a distance less than an extrinsic Debye length: 1 LD = ( (a) kT 2 ) q p (9) s o 2 where q is the electron charge, and the measured apparent hole concentration is an average p(x) taken over a distance of this order [6] Rewriting Eq. (8), replacing w with x, and N(w) with p(x) to mathematically relate the measured capacitance Cm of the MNOS structure and the majority carrier distribution p(x): 1 ) Cm2 ] dV d( p ( x) = 2[q (b) Fig. (1) (a) ideal MNOS structure, (b) ideal HF, LF and deep depletion (DD) C-V curves In our case, the nitride layer thickness is about 50 times greater than silicon dioxide layer thickness; we can approximate Eq. (1) to: (4) Ci = Cn Hence, the measured MNOS capacitance (Cm) is equal to: CC (5) Cm = n d Cn + Cd C + Cn (6) Cd = m Cn Cm where Cd is the depletion capacitance and given by: o (7) w where w is the depletion width and s is silicon relative dielectric constant (=11.9) The depletion capacitance changes with voltage from a maximum at which the total capacitance is equal to Cn, toward a minimum of Cmin when the depletion depth is maximum wm, and the capacitance curve reach its minimum Cmin, Fig. (1b). We can calculate Cdmin from the C-V curve at Cmin by substituting the value of Cmin in Eq. (6) and calculating Cd equals to Cdmin [11]. The depletion approximation method of doping profile is [7]: 1 d( 2 ) 3 Cm Cm dC ]1= ( m ) 1 (8) N ( w) = 2[q s o dV q o s dV Cd = 36 s s o 1 (10) Following the derivation in [12], by introducing the effect of stretch out of C-V curve caused by interface states, the interface states corrected hole profile p'(x) is obtained: 1 C LF d( 2 ) 1 Cn Cm 1 (11) )[q s o ] p' ( x) = 2( C HF dV 1 Cn Kennedy et al. [13] developed a simple mathematical formula which expresses the doping as a function of free carrier concentration in one dimension, following their derivation but for holes rather than electrons because electrons were their majority carriers: The electric current within this material due to both drift and diffusion of majority holes is given by: dp d1 (12) J p = qD p qpµ p dx dx where Jp is hole current density, Dp is holes diffusion constant, µp is holes mobility, and 1 is the electric potential Einstein relation states that: Dp µp = kT q (13) An electric current of zero implies that the diffusion and drift terms in Eq. (12) are of equal magnitude, but in the opposite direction; hence, from equations (12) and (13), an electric field E(x) is obtained: d1 kT 1 dp( x) (13) E ( x) = = dx q p( x) dx where k is Boltzmann’s constant, and T is absolute temperature Equation (14) establishes the electric field distribution necessary to maintain an electric current of zero in p-type material containing local variations of holes density. Assuming © 2010 Iraqi Society for Alternative and Renewable Energy Sources and Techniques (I.S.A.R.E.S.T.) Iraqi Journal of Applied Physics extrinsic semiconductor material (the minority carrier density has negligible influence upon the structure under consideration), we have from Poisson’s equation q dE (15) = [ p ( x) N a ( x)] dx s o The divergence of the electric field, in Eq. (14) is determined by both the impurity atom distribution Na(x) and the majority carrier distribution p(x), by combining equations (14) and (15) we obtain: kT d 1 dp ( x) q { }= [ N a ( x) p ( x)] (16) q dx p ( x) dx s o and therefore kT d 1 dp ( x) (17) N a ( x) = p ( x) ( s o )( ) [ ] q q dx p ( x) dx Equation (17) rigorously relates the desired impurity atom distribution Na(x) to the measured majority carrier distribution p(x). In order to extend doping profile deeper inside the silicon, we must obtain deep depletion DD C-V curve. When the gate bias is swept from accumulation into the inversion region too fast for minority carrier (electrons) to follow, the charge neutrality must be satisfied by the ionized acceptor alone, therefore, the depletion width become broader than that in thermal equilibrium, and the capacitance decreases below its thermal equilibrium saturation value (Cinv). Such a nonequilibrium condition is called deep depletion [14]. Usually deep depletion can be achieved by increasing the voltage bias sweep rate in the C-V measurement (high enough that not allow the creation of minority electrons). 3. Material and experimental technique The measured device is MNOS structure. ptype (100) silicon wafer of resistivity 5-10 2.cm is used with approximately doping of about 2x1015cm-3. Native SiO2 layer of thickness ~2nm is formed, Si3N4 layer is deposited by using of Low Pressure Chemical Vapor Deposition (LPCVD) method, the thickness is 171nm measured by ellipsometry. Aluminum is used as front and back contacts. The front contact is deposited at low pressure of 5x10-6 mbar across suitable mask of area 0.01cm2 using Edward 306 A coating system. The back contact is deposited without mask. Two methods of C-V measurements are performed: (1) The conventional C-V measurement is performed on FLUKE PM 6306 programmable Automatic RLC Meter. The voltage sweep bias is supplied by Keithly Pico-Ammeter/DC Voltage Source Model 6487. Electrical contacts are made by pressing the metallic gate using a spring clip arrangement. All rights reserved (2) The DD C-V measurement is achieved by the application of high speed saw tooth voltage on MNOS sample provided by TEKTRONIX FG 502-11MHz Function Generator. The DD C-V curve is traced on the screen of TEKTRONIX (1GHz) TDS 5104 Digital Phosphor Oscilloscope, which has the ability of saving and exporting the wave form to MATLAB for mathematical operations. The voltage bias is supplied by the same previous Kiethly DC voltage source for returning flat-band voltage to the origin of the scope's screen. Whole measurements are performed in dark at room temperature 300K. A full description of this circuit with an example of C-V curve as shown on the CRO screen is given in the appendix. 4. MATLAB (6.5) Algorithm The following MATLAB Algorithm is designed for the determination of doping profile 5. Results and Discussion Figure (2) shows the 1MHz C-V curve of MNOS sample, in which the scan is initiated at voltage of -20V in accumulation mode towards the inversion with sweep rate of =3V/s. Nitride's capacitance per unit area Cn is calculated from the accumulation and its equal to 2.375x10-8F/cm2. The flat-band voltage (VFB) is ISSN 1813-2065 Printed in IRAQ 37 IJAP Vol. (6), No. (1), January 2010 standard LF C-V curve. The shape of C-V curve, whether it takes HF or LF shape, depends on minority carriers lifetime [9]. When the life time is long, the C-V curve takes LF shape in very low frequencies, as low as possible; to the degree the minority carriers could follow the ac signal, i.e., quasi-static. But as we will show later, it is obvious that minority carrier life time is so small that we have LF C-V curve even at 10 kHz. also calculated and it is equal to -16.8V using 0.9Cacc rule. The rule which states that: flat band capacitance CFB is equal to 90% of accumulation capacitance Cn [15]. 5.1 Deep Depletion It is necessary to extend the profile deeper inside the silicon substrate in order to get more accurate information about doping concentration change with depth, and thus for: first, the conventional doping profile is limited to small depths inside the silicon - that is, calculated in our case as 0.6µm, and valuable information about the exact doping can not be achieved in such small depths. Second, the change in majority carriers, actually measured by C-V profiling, limits the resolution of the differential capacitance method to distances comparable to the local extrinsic Debye length [6,19]. We calculate LD using Eq. (9) for NA=2x1015cm-3, as 0.09µm. Figure (4) shows LF (10 kHz), HF (1MHz), and DD C-V curves. The DD C-V curve is obtained by using the circuit given in the appendix. The transient C-V curve can be achieved directly by measuring MNOS current response to a very fast voltage ramp of sweep rate of 1MV/s, this current response is proportional to the differential capacitance and carries information on the doping density [8]. Thus, as it was mentioned previously, the large sweep rate ( =106V/s) indicates that the minority carrier life time is very small [12]. Fig. (2) C-V curve of MNOS sample under the application of voltage ramp of sweep rate (3V/s) from accumulation (-ve voltages) to deep inversion (+ve voltages), and then in the reverse direction The curve which shows an increase of capacitance in strong inversion as a result of formation of certain amount of interface state tarps because of the large DC field stress ~1.2x106V/cm [16,17], then we record a constant capacitance till the end of the scan(+40V), like an ideal C-V curve. In the reverse direction we notice two effects: the first one is another increase of capacitance as a result of creation of interface state traps; the second one is that we get the flat–band condition at +7V, this results in a memory window of 23.8V, which indicates that electrons are tunneled across the silicon dioxide and then trapped in the silicon nitride layer [18]. Figure (3) is the conventional C-V curves of MNOS capacitors at frequencies (10 kHz, 100 kHz and 1 MHz), the DC sweep rate is the same for all frequencies =3V/s. 300 Capacitance (pF) 200 100 10KHz 100KHz 1MHz 0 -25 -20 -15 -10 Voltage (V) -5 0 Fig. (3) Three C-V curves at 10 kHz, 100 kHz and 1MHz. The sweep rate is the same (3V/s) The 10kHz curve shows an increase in the inversion capacitance toward Cn like the case of 38 Fig. (4) Three MNOS C-V curves 10 kHz, 1 MHz and DD, the sweep rate for the first two curves is the same (3V/s), while for DD curve it is 1MV/s 5.2 Calculation of Doping Profile The majority hole profile from the surface toward the bulk of p-type silicon substrate is calculated by Eq. (10) using conventional C-V, © 2010 Iraqi Society for Alternative and Renewable Energy Sources and Techniques (I.S.A.R.E.S.T.) Iraqi Journal of Applied Physics and DD curves as its shown in Fig. (5). DD C-V profile provides additional 1µm deeper inside the silicon compared to the conventional differential C-V profile. At onset of inversion, the calculation of hole profile is not accurate [12], that is why we see a rapid increase of hole density. seemed to be an average of charge density profile. The interface state correction terminates at about 0.6µm because the LF C-V measurement's lowest capacitance is 1.096*10-8 F/cm2 corresponds to depletion width of 0.6µm by using equations (5) and (6), while the lowest DD capacitance is at 0.52x10-8F/cm2 corresponds to depletion width of 1.5µm, that is why we cannot extend the interface state correction of hole profile p'(x) to distances greater than 0.6µm. Fig (5) Hole profile using (1MHz) equilibrium and deep depletion (DD) method Figure (6) shows the comparison between the interface state density correction of hole profile p'(x) using Eq. (11) with hole profile p(x). The two are approximately of the same value, therefore we can ignore the effect of interface state in our calculations. The graph shows a decrease in hole density when we go deeper inside the silicon which is similar to the change in doping density calculated from Eq. (17), as it is shown in Fig. (7). Fig. (6) Hole profile p(x) and interface states corrected hole profile p'(x) In this curve p(x), p'(x) and the doping densities Na(x) reach approximately a constant value of about 2x1015cm-3. The reason behind the change in doping at the surface is that thermal oxidation of silicon moves dopant ions from their equilibrium positions [12]. Moreover, the thermal deposition of the Si3N4 layer may cause additional rearrangement of the dopant ions. Deeper inside the silicon, the hole density is All rights reserved Fig. (7) Doping profile Na(x), and hole profile p(x) 6. Conclusions C-V technique gives suitable information about impurity charge distribution near and the surface of silicon substrate of MNOS device. A deep depletion DD MNOS C-V curve was obtained by the application of high speed voltage ramp of sweep rate of (106V/s), and the current response of such voltage ramp is monitored. It was found that interface states densities have negligible effect on the calculation of doping profile. Doping profile decrease with going deep into the silicon bulk reaching approximately a constant value of 2x1015cm-3. References [1] J.R. Elmiger and M. Kunst, Appl. Phys. Lett., 69(4) (1996) 517-519. [2] T.P. Ma, IEEE Trans. Electron Devices, 45(3) (1998) 680-690. [3] J. Heo et al., Mater. Sci. and Eng. B, 124125 (2005) 301-304. [4] A. Pirovano et al., IEEE Trans. Electron Devices, 48(4) (2001) 750-757. [5] F. Recart and A. Cuevas, IEEE Trans. Electron Devices, 53(3) (2006) 442-448. [6] H. Kroemer and W.Y. Chien, Solid State Electron., 24 (1981) 655-660. [7] A.F. Yaremchuk, Appl. Phys. A, 73 (2001) 503-509. [8] R.C. Hughes, R. Bastasz and W.P. Ellis, Appl. Surf. Sci., 115 (1997) 74-79. [9] R.F. Pierret, "Semiconductor Device Fundamentals", Addison-Wesley ISSN 1813-2065 Printed in IRAQ 39 IJAP Vol. (6), No. (1), January 2010 Publishing Co., Inc. (USA) (1996), Ch. 16, 587-591, 595-598. [10] S.M. Sze, "VLSI Technology", McGrawHill Book Co. (Singapore) (1988), Ch. 6, 259-263. [11] S.M. Sze and K.N. Kowk, "Physics of Semiconductor Devices", John-Wiley & Sons, Inc. (NJ, USA) (2007), Ch. 4, 202209. [12] E.H. Nicollian and J.R. Brews, "MOS Metal Oxide Semiconductor Physics and Technology", John-Wiley & Sons, Inc. (NJ, USA) (2003) Ch. 9, 387-390, 375-380, Ch. 14, 721-731. [13] D.P. Kennedy and R.R. O'Brien, IBM J. Res. Develop., (1968) 212-214. [14] C.Y. Liu, B.Y. Chen and T.Y. Tseng, J. Appl. Phys., 95(10) (2004) 5602-5607. [15] D.K. Schroder, "Semiconductor Material and Device Characterization", John-Wiley & Sons, Inc. (NJ, USA) (2006), Ch. 6, 328. [16] S. Minami and Y. Kamigaki, IEEE Trans. Electron. Devices, 40(11) (1993) 2011-2017. [17] C. Bae, "GaN-dielectric interface formation for gate dielectrics and passivation layers using remote plasma processing", Ph.D. Thesis, North Carolina State University, (USA) (2003). [18] K. Ohnishi, and K. Miura, Electron. and Commun. in Japan, part 2, 75(4) (1992) 5259. [19] C.L. Wilson, IEEE Trans. Electron. Devices, 27(12) (1980) 2262-2267. Appendix Fast ramp (1MV/s) C-V tracer circuit with a snapshot of the CRO screen dv =constant dt The capacitance C = dq = dq dt = i dv dt dv The sweep rate = (a1) (a2) Where i is the instantaneous current, hence the i-v curve shown on the CRO screen can be converted into C-V curve using Eq. (a2) _____________________________________________________________________________________ 40 © 2010 Iraqi Society for Alternative and Renewable Energy Sources and Techniques (I.S.A.R.E.S.T.)